3.
Monte Carlo andMolecular Dynamics Simulations in Polymer Science KURT BINDER Institut fur Physik Johannes-Gutenberg- Universitdt Mainz New York Oxford OXFORD UNIVERSITY PRESS 1995
5.
PREFACEComputer simulation has become an established method of research inscience and a useful tool in solving certain engineering problems. With theintroduction of powerful workstations on the desk of the scientist, theimpact of the application of computer simulation to many problems willincrease enormously in the next couple of years. Polymer science profits from this development in a particular way: thecomplexity of macromolecular chemical architecture and geometrical struc-ture, the huge variability of physical properties and the widespread range ofapplications involves many intricate scientific questions, considering the factthat theoretical methods usually imply crude mathematical approximations,the validity of which it is hard to judge in general. Together with the limita-tion that unknown parameters introduce, the predictive power of such workis often rather limited. In contrast, computer simulation can study a modelof a complex many-body system in full detail without invoking such math-ematical approximations: in principle, we thus can check the validity ofapproximate calculations and methods, without unknown parametersobscuring a meaningful comparison. At the same time, comparing withexperiment helps to validate and systematically improve the model. Infact, use of computer simulation in this way is an iterative process bywhich the understanding of complex materials and processes can be signifi-cantly improved step by step. In view of these distinct conceptual and principal advantages, computersimulations in macromolecular materials have aroused considerable interest,and various complementary techniques have been developed. It must benoted, though, that simulations of polymers pose particular challenges, con-sidering the enormous spread of length scales and time scales involved: eventhe simple case of a single flexible polyumer coil exhibits geometrical struc-ture from the scale of a chemical bond (1A) to the scale of the gyrationradius (100A), and collective length scales in dense materials often are evenmuch larger. Simultaneously, times scales range from bond vibration times(10"13 sec) to macroscopic times (103 sec), characterizing interdiffusion orrelaxation near the glass transition, etc. Hence the naive use of "molecularmodeling" software packages as a "black box" cannot be relied upon as aproblem solver — what is needed, of course, is a more basic understandingof what computer simulation is, what methods are implemented and wheretheir strengths and limitations lie. It is one of the aims of the present book toprovide the reader with such background knowledge, which will enable himto apply such software with mature judgement in a useful way. Some of the
6.
vi PREFACEchapters of this book therefore discuss deliberately methodical aspects ofMonte Carlo and molecular dynamics simulations and describe the role of"model building". Given the inevitable uncertainties about the force fieldsfor complex polymeric materials, and the difficulty in explicitly relatingthese forces and other details of the geometrical and chemical structure tophenomenological simplified models, the book pays much attention to thequestion "which model is adequate for a considered problem?" and clearlydistinguishes questions where one can obtain sensible answers from simula-tions from those where one cannot. The emphasis of this book is on polymer physics rather then polymerchemistry, and it considers in the main amorphous polymers (in solution,melt, or solid state); crystallized polymers, as well as polymer crystallizationprocesses, etc., are not discussed here, nor are biopolymers treated—although many of the general comments about polymer simulation thatcan be found in this book are presumably useful for these other fields aswell. Such a restriction of scope was necessary in order to keep the length ofthe text manageable. Taking the input from quantum chemistry (force fields,etc.) as given wherever necessary, the book does contain chapters dealingwith fairly realistic models containing much chemical detail (e.g., the chap-ter by J.H.R. Clarke on simulations of the elastic properties of glassy poly-mers and that by D.Y. Yoon et al. on interfacial properties in thin polymericlayers). Most of the book, though, deals with more "mesoscopic" proper-ties, attempting to bridge the gap between atomistic structure and macro-scopic properties: structure and elastic response of polymer networks, forcesacting between polymer brushes, phase diagrams of polymer blends, etc. Ofcourse, the structure and dynamics of polymer coils under the various con-ditions is a central theme that can be found in almost all chapters: Chapter 2describes what is known about the treatment of excluded volume interactionin dilute solution; Chapter 3 emphasizes electrostatic and hydrodynamicforces; stretching of chains in deformed rubbers is discussed in Chapter 4;stretching of chains due to thermodynamic forces in block copoymer meso-phases in Chapter 7; and of tethered chains in Chapter 9. Thus, a widevariety of problems encountered with synthetic polymers is addressed.Studying the book will give a broad overview of almost the complete fieldof polymer physics and its concepts; and thus certainly will be useful tostudents and researchers in that field. Besides providing such an introduc-tion, it presents up-to-date reviews from the leading experts on the variousapplications that are covered here, and it is expected that it will play astimulating role in research, pushing further the frontier of new develop-ments in academia and industry.Mainz, September 1994 Kurt Binder
7.
CONTENTS1. Introduction: General Aspects of Computer Simulation Techniques and their Applications in Polymer Physics KURT BINDER 1.1 Why is the computer simulation of polymeric materials a challenge? 3 1.1.1 Length scales 3 1.1.2 Time scales 7 1.2 Survey of simplified models 10 1.2.1 Off-lattice models 10 1.2.2 Lattice models 14 1.3 Taking the idea of coarse-graining literally 19 1.3.1 Effective potentials for the bond fluctuation model 19 1.3.2 How different coarse-grained models can be compared 22 1.4 Selected issues on computational techniques 28 1.4.1 Sampling the chemical potential in NVT simulations 28 1.4.2 Calculation of pressure in dynamic Monte Carlo methods 34 1.5 Final remarks 39 References 412. Monte Carlo Methods for the Self-Avoiding Walk ALAN D. SOKAL 2.1 Introduction 47 2.1.1 Why is the SAW a sensible model? 47 2.1.2 Numerical methods for the self-avoiding walk 49 2.2 The self-avoiding walk (SAW) 51 2.2.1 Background and notation 51 2.2.2 The ensembles 55 2.3 Monte Carlo methods: a review 56 2.3.1 Static Monte Carlo methods 57 2.3.2 Dynamic Monte Carlo methods 60 2.4 Static Monte Carlo methods for the SAW 65 2.4.1 Simple sampling and its variants 65 2.4.2 Inversely restricted sampling (Rosenbluth-Rosenbluth algorithm) 69 2.4.3 Dimerization 70 2.5 Quasi-static Monte Carlo methods for the SAW 73 2.5.1 Quasi-static simple sampling 73 2.5.2 Enrichment 73 2.5.3 Incomplete enumeration (Redner-Reynolds algorithm) 75 2.6 Dynamic Monte Carlo methods for the SAW 77
8.
viii CONTENTS 2.6.1 General considerations 77 2.6.2 Classification of moves 79 2.6.3 Examples of moves 81 2.6.4 Fixed-./V, variable-x algorithms 85 2.6.5 Fixed-N, fixed-x algorithms 94 2.6.6 Variable-TV, variable-* algorithms 95 2.6.7 Variable-jV, fixed-* algorithms 98 2.7 Miscellaneous issues 101 2.7.1 Data structures 101 2.7.2 Measuring virial coefficients 105 2.7.3 Statistical analysis 106 2.8 Some applications of the algorithms 108 2.8.1 Linear polymers in dimension d = 3 108 2.8.2 Linear polymers in dimension d = 2 113 2.9 Conclusions 114 2.9.1 Practical recommendations 114 2.9.2 Open problems 114 References 1173. Structure and Dynamics of Neutral and Charged Polymer Solutions: Effects of Long-Range Interactions BURKHARD DUNWEG, MARK STEVENS, and KURT KREMER 3.1 Introduction 125 3.2 Dynamics of neutral polymer chains in dilute solution 127 3.2.1 Theoretical background 129 3.2.2 Simulations 134 3.3 Structure of charged polymer solutions 159 3.3.1 Theoretical models 162 3.3.2 Experiment 167 3.3.3 Simulation methods 168 3.3.4 Simulation results 172 3.4 Conclusion 186 References 1884. Entanglement Effects in Polymer Melts and Networks KURT KREMER and GARY S. GREST 4.1 Introduction 194 4.2 Theoretical concepts 199 4.2.1 Unentangled melt 200 4.2.2 Entangled melt 203 4.3 Model and method 211 4.4 Simulations of uncrosslinked polymers 217 4.4.1 Reptation simulations 217
9.
CONTENTS ix 4.4.2 Melt simulations on a "molecular level" 221 4.4.3 Comparison to experiment 233 4.4.4 Semidilute solutions 237 4.5 Polymer networks 242 4.5.1 Network elasticity 243 4.5.2 Networks with fixed crosslinks 245 4.5.3 Fully mobile systems 247 4.6 Conclusions 259 References 2625. Molecular Dynamics of Glassy Polymers JULIAN H. R. CLARKE 5.1 Introduction 272 5.2 Molecular dynamics for polymers 274 5.3 Force fields 276 5.4 Preparation of polymer melt samples 279 5.4.1 Building polymer structures 279 5.4.2 Introducing excluded volume 280 5.4.3 Sample relaxation 281 5.4.4 Sample size effects 283 5.5 Preparation of polymer glasses 283 5.5.1 Glass preparation by computer simulation 283 5.5.2 The glass transformation on different time scales 286 5.6 Stress-strain properties 289 5.6.1 Uniaxial tension simulations 289 5.6.2 Stress-strain behavior and configurational properties 295 5.7 Penetrant diffusion 299 5.8 Local motions in amorphous polymers 302 References 3046. Monte Carlo Simulations of the Glass Transition of Polymers WOLFGANG PAUL and JORG BASCHNAGEL 6.1 Introduction 307 6.2 Model and simulation technique 312 6.2.1 The definition of the bond fluctuation model 312 6.2.2 Hamiltonians and cooling procedures 313 6.3 Results for the schematic models 315 6.3.1 Structural properties of the melt 318 6.3.2 Dynamic properties of the melt 332 6.4 Modeling of specific polymers 344 6.4.1 How to map naturalistic models to abstract models 344 6.4.2 Modeling bisphenol-A-polycarbonate 347 6.5 Summary 351 References 353
10.
x CONTENTS7. Monte Carlo Studies of Polymer Blends and Block Copolymer Thermodynamics KURT BINDER 7.1 Introduction 356 7.2 Simulation methodology 362 7.2.1 Dynamic algorithms and the role of vacancies 362 7.2.2 The semi-grand-canonical technique for polymer blends 364 7.2.3 Other ensembles 372 7.2.4 Finite size scaling 375 7.2.5 Technical problems of simulations of block copolymer mesophases 382 7.2.6 Interfacial structure, surface enrichment, interdiffusion, spinodal decomposition 391 7.3 Results for polymer blends 395 7.3.1 Test of the Flory-Huggins theory and of the Schweizer-Curro theory 396 7.3.2 Critical phenomena and the Ising-mean field crossover 401 7.3.3 Asymmetric mixtures 402 7.3.4 Chain conformations in blends 405 7.3.5 Interdiffusion and phase separation kinetics 407 7.3.6 Surfaces of polymer blends and wetting transitions 409 7.4 Results for block copolymers 415 7.4.1 Test of the Leibler theory 415 7.4.2 Chain conformations and the breakdown of the random phase approximation (RPA) 417 7.4.3 Asymmetric block copolymers; ring polymers 420 7.4.4 Block copolymers in reduced geometry: thin films, interfaces, etc. 422 7.5 Discussion 423 References 4268. Simulation Studies of Polymer Melts at Interfaces D. Y. YOON, M. VACATELLO, and G. D. SMITH 8.1 Introduction 433 8.2 Systems of atomistic chains 434 8.2.1 General considerations 434 8.2.2 Models and methods 435 8.2.3 Liquid «-tridecane near impenetrable walls by Monte Carlo simulations 441 8.2.4 JV-Alkane systems near neutral and attractive surfaces by SD and MD simulations 445 8.2.5 Liquid tridecane in a narrow and a broad slit in equilibrium 453 8.2.6 Systems with free surfaces 457
11.
CONTENTS xi 8.2.7 Explicit atom simulations of «-alkanes at interfaces 461 8.2.8 Comparison of atomistic simulations with Scheutjens-Fleer lattice theory 464 8.3 Systems of bead chains 466 8.3.1 General considerations 466 8.3.2 Models and methods 467 8.3.3 Results 469 8.4 Conclusions 473 References 4749. Computer Simulations of Tethered Chains GARY S. GREST and MICHAEL MURAT 9.1 Introduction 476 9.2 Models and methods 479 9.2.1 Lattice models 480 9.2.2 Off-lattice models 485 9.2.3 Numerical solution of SCF equations 492 9.3 Polymers tethered to a point 494 9.3.1 Star polymers in a good solvent 497 9.3.2 Star polymers in a 6 and poor solvent 502 9.3.3 Relaxation of star polymers 506 9.4 Polymers tethered to a line 509 9.4.1 Polymers tethered to an inflexible line 510 9.4.2 Polymers tethered to a flexible line 513 9.5 Polymeric brushes 514 9.5.1 Brushes in good solvents 516 9.5.2 Brushes in 6 and poor solvents 526 9.5.3 Attractive grafting surfaces 532 9.5.4 Polydispersity effects 534 9.5.5 Interaction between brushes 535 9.5.6 Brushes on curved surfaces 541 9.5.7 Brushes without a solvent 545 9.5.8 Time-dependent phenomena 547 9.6 Polymers tethered to themselves 551 9.6.1 Flory theory 552 9.6.2 High-temperature flat phase 555 9.6.3 Effect of attractive interactions 563 9.7 Conclusions 565 References 566 Index 579
13.
CONTRIBUTORSJorg Baschnagel Kurt KremerInstitutfur Physik Institut fur FestkorperforschungJohannes- Gutenberg- Un iversitdt Forschungszentrum Jiilich Mainz Postfach 1913 WA 331/339 D-52425 JiilichD-55099 Mainz GermanyGermany Michael MuratKurt Binder Department of Physics and AppliedInstitutfur Physik MathematicsJohannes-Gutenberg-Universitdt Soreq Nuclear Research Center Mainz Yavne 70600 WA 331J339 IsraelD-55099 MainzGermany Wolfgang Paul Institutfur Physik Johannes-Gutenberg-UniversitdtJulian H. R. Clarke MainzChemistry Department WA 331/339University of Manchester D-55099 MainzInstitute of Science and Technology GermanyPO Box 88Manchester M60 1QD Grant. D. SmithU.K. Department of Chemical Engineering University of Missouri-ColumbiaBurkhard Dunweg Columbia, MO 65211Institutfur PhysikJohannes-Gutenberg-Universitdt Alan D. Sokal Mainz New York University WA 331/339 Department of PhysicsD-55099 Mainz 4 Washington PlaceGermany New York, NY 10003Gary S. Grest Mark StevensCorporate Research Science Corporate Research Science Laboratories LaboratoryExxon Research and Engineering Co. Exxon Research and Engineering Co.Annandale, NJ 08801 Annandale, NJ 08801
14.
xiv CONTRIBUTORSM. Vacatello D.Y. YoonDepartment of Chemistry IBM Research DivisionUniversity of Naples Almaden Research CenterVia Mezzocannone 4 650 Harry Road80134 Napoli San Jose, CA 95120-6099Italy
15.
MONTE CARLO AND MOLECULAR DYNAMICS SIMULATIONS IN POLYMER SCIENCE
17.
1 INTRODUCTION: GENERAL ASPECTS OF COMPUTER SIMULATION TECHNIQUES AND THEIR APPLICATIONS IN POLYMER PHYSICS Kurt Binder1.1 Why is the computer simulation of polymeric materials a challenge?In recent years computer simulation has become a major tool in polymerscience, complementing both analytical theory and experiment. This interestis due both to the many fundamental scientific questions that polymer sys-tems pose and to the technological importance of polymeric materials. Atthe same time, computer simulation of polymers meets stringent difficulties,and despite huge progress (as documented in previous reviews1"7) manyproblems are still either completely unsolved or under current study. Inthe following pages these difficulties are briefly discussed.1.1.1 Length scalesFor standard problems in the physics and chemistry of condensed matter,such as simple fluids containing rare gas atoms or diatomic molecules, etc.,computer simulation considers a small region of matter in full atomisticdetail.8"13 For example, for a simple fluid it often is sufficient to simulatea small box containing of the order of 103 atoms, which interact with eachother with chemically realistic forces. These methods work because simplefluids are homogeneous on a scale of 10 A already; the oscillations in thepair distribution function then are damped out under most circumstances.Also reliable models for the effective forces are usually available from quan-tum chemistry methods. For long flexible polymers we encounter a different situation (Fig. l.l)14:already a single chain exhibits structure from the scale of a single chemicalbond (w 1 A) to the persistence length15 (w 10 A) to the coil radius («100 A). Additional length scales occur in a dense polymer solution ormelt. Some of these length scales are smaller than the coil radius, such asthe screening length £ev in semidilute solutions,16 which describes the rangeover which excluded volume forces are effective, or the tube diameter inmelts,17 which constrains the motion of a chain (due to entanglements withother chains) in a direction along its own (coarse-grained) contour (seeChapter 4, where estimation of this length from simulations is discussed).
18.
4 INTRODUCTIONFig. 1.1 Length scales characterizing the structure of a long polymer coil (polyethylene is usedas an example). (From Binder.14)Collective phenomena may even lead to much larger lengths: e.g., in apolymer brush (i.e., a layer of polymers anchoring with a special endgroup at an otherwise repulsive wall) the height h of the brush is predictedto scale with degree of polymerization Np as18 h oc Np, while the coil gyra-tion radius Rs scales only as Rg oc ^/N^ in a 0-solution or dense melt1619 orRg oc A^ with v zi 0.59 in a good solvent.1620 Thus for 7VP of the order 103 to104 and a sufficiently high grafting density one expects h to be of order 103 A(see also Chapter 9, where the simulation of polymer brushes is treatedfurther). Another large length scale occurs in polymer blends near the critical pointof unmixing, namely the correlation length £ of concentration fluctuations.21One expects that this length is of the order of R&, far away from the criticalpoint, but approaching the spinodal curve it is enhanced by a factor|1 - r/r sp (^)p 1/2 , where Tis the temperature of the blend and T^(<j>) thespinodal temperature at volume fraction <j> of one component of the blend.This enhancement factor is a mean-field result,162122 and close to thecritical temperature Tc one expects an even faster growth of critical correla-tions,2123 f oc ^"^(T/Tc - I)""1, where ^ « 0.63 is the Ising model cor-relation length exponent24 and a the size of a segment of the polymer chain.Thus, near Tc correlation lengths of the order of 103 A are predicted21"23 andobserved25. Similar large length scales are predicted2122 and observed212627in the spinodal decomposition of polymer blends that are quenched into theunstable region of the phase diagram and hence start phase separation (seealso Chapter 7, where the simulation of polymer blends is treated further).
19.
COMPUTER S I M U L A T I O N OF P O L Y M E R I C M A T E R I A L S 5 This list of characteristic lengths in polymeric materials is far from beingexhaustive. Without detailed explanation we here simply mention also thecharacteristic thickness of lamellae A ex aNp in the strongly segregatedlamellar mesophase of block copolymers,28 the Bjerrum length, the electro-static persistence length, and the Debye-Hiickel screening length in poly-electrolyte solutions29"32 (see Chapter 3 for simulations of such systems), thedistance between crosslinks in polymer networks (see Chapter 4), character-istic coil sizes of polymers exposed to shear flow,33 and so on. Since a valid computer simulation must choose a system size with lineardimensions L larger than the characteristic lengths of the problem, one findsthat for many problems of interest one would need to simulate systemscontaining of the order of at least 106 atoms or even much more. Thesituation becomes aggravated since the effective potentials for polymersare much more complicated and hence difficult to use in simulations thanthe pair potential for simple fluids. Let us consider polyethylene (PE), thechemically simplest organic polymer, as an example. A very popular modelignores the hydrogen atoms of the (CH2) groups and replaces them withunited atoms34""*4 (Fig. 1.2; see also Chapter 5 for more details). Neither thebond lengths nor the bond angles in Fig. 1.2 are treated as rigid, and oneuses harmonic potentials for bond length and bond angle vibrations, whilenonbonded interactions between effective monomers of different chains (ormonomers of the same chain if they are separated by more than three bondsalong the chain) are represented by a Lennard-Jones form. Thus already forthe simplified model of Fig. 1.2 a complicated Hamiltonian with manyparameters results:whereThe appropriate choice of the parameters fy, to, fe, cos6o, f<s>, a,... ,as(a0 = 1), c and <r is discussed in the literature34^5: at this point we notethat even for the torsional potential 3f^($j) and the nonbonded interactionJ^LJ there is no complete agreement between different authors. Thus formany other polymers where the monomers are chemically more complicatedthe force fields are even less well known. Furthermore, the nonbondedinteraction for computational convenience is often truncated at rathershort distances ry between monomers i, j such as39 ry = 1.5cr; experience
20.
6 INTRODUCTIONFig. 1.2 (a) Schematic model of a piece of the polyethylene chain. The hydrogen atoms (H) arenot treated explicitly in the "united atom" approximation, but rather one introduces effectivespherical segments (shaded) representing a whole CH2 unit. The segments are connected byharmonic bonds (shown as straight lines), the bond lengths being it (segments being labeledconsequently by an index i, i = 0 to Nv — 1). Three successive segments ; — 1, i, i+ 1 define abond angle 6; and four successive segments {; — 2, i - 1,;,/ + 1} a torsional angle fa, namely theangle between the plane spanned by the bonds formed from the segments {i — 2, z — 1, i} and theplane built from {i - 1, i, i+l}. Note that the fa values are zero in the all-trans configurationdrawn here, (b) Qualitative sketch of the torsional potential for alkane chains, indicating thethree energetically prefered states, gauche- (g~), trans (t), and gauche + (g+). The minimum ofthe trans configuration is deeper by an amount Af7. (From Kremer and Binder.2)with monatomic fluids46 shows that the equation of state of the fluid israther sensitive to the value of this cut-off. Note that usually no distinctionis made for the CHj, end-groups of the chain. In view of this discussion, it is clear that even the detailed model ofeqs (!.!)-(1.3) should not be taken as a faithful description of polyethylene(PE), but rather as a prototypical schematic model of linear polymers. In thecontext of simulations of lipid monolayers,47 it has been suggested that it isnecessary to shift the center of gravity of the united atom off the position ofthe carbon atom at the chain backbone (anisotropic united atom model).Very recent work48 (see also Chapter 8) suggests that it is more satisfactoryto include the hydrogen atoms explicitly, if one wishes to describe PE prop-erly. For the reasons quoted above, such work is restricted to relatively
21.
C O M P U T E R S I M U L A T I O N OF P O L Y M E R I C M A T E R I A L S 7small degree of polymerization Np, and thermodynamic states far off fromany phase transitions.1.1.2 Time scalesWhen one considers the second factor that controls simulation feasibility,namely the time scales involved, one realizes that the situation is evenworse. While in simple fluids at states far from phase transitions all fluctua-tions decay on time scales of a few picoseconds, and hence moleculardynamics (MD) simulations can easily produce well-equilibrated system con-figurations, this is not so for polymers, since motions occur on many verydifferent time scales. Fast motions such as the vibrations of the length t of aC-C bond (Fig. 1.2) or the bond angle 0 (Fig. 1.2) may take times of the orderof Tvjb PS 10~13 s or even less. However, already the reorientation jumps in thetorsional potential (t <-> g+, g_; Fig. 1.2) are significantly slower; the averagetime T between two such jumps is typically of the order of r w 10~n s, forpolymer melts at the temperatures of interest. Since the time integration stepSt of a MD simulation has to be much smaller than the shortest characteristictime, it has become common to either take the bond length as rigid38 or tosoften the spring constant/^ in eq. (1.2) by a factor of seven arbitrarily,39"*2 toalleviate this problem. Using 10 chains with Np = 50, a time-step ofSt = 10~14s has been chosen39 and a CPU time of 0.02s on a CRAY-XMPsupercomputer was reported.39 Thus, even at high temperatures far above theglass transition one needs 20 s to have a single jump in the torsional potential,and near the glass transition—where T increases proportional toTI oc Tvjb exp(AE/ksT), A£ being the energy barrier of the torsional potentialin Fig. 1.2—even a much longer simulation would hardly observe any t ^ g+,g_ transitions. It should also be noted that the choice of St = 10~14 s is ratherlarge, which may also lead to uncontrolled errors (other work38 makes themore conservative choice of 6t = 2.10~15 s). Choosing MC instead of MD toequilibrate the system configurations is of little help here, however, since formost MC moves the acceptance rates are very small. Of course, having just a few jumps in the torsional potential suffices toproduce equilibrium on a very short length scale, but is not enough to bringthe persistence length and the gyration radius Rg to their equilibrium values.Let us assume that we deal with a melt of relatively short, nonentangledchains, i.e., Np < Nep where typically17 Nep PS 102, so that the Rouse model17holds. Then the relaxation time necessary to relax the global configurationof a coil (Fig. 1.1) varies asThus for Np PS 30 a relaxation time rNv « 10~8 s results, 106 times more thanthe time-step of Rigby and Roe.39 This number shows that even at high
22.
8 INTRODUCTIONtemperatures it is at best possible to equilibrate melts of very short chains,and this indeed has recently become feasible.48 (see also Chapter 4 for amore detailed discussion). Of course, the situation is much worse for melts of long chains in amutually entangled state, where reptation theory1617 predicts a relaxationtime proportional to the third power of N,For Np = 500 one then estimates that rNp at 10 5 s, eight orders of magnitudemore than the vibration time rv(b! Therefore a straightforward application ofMD to study the dynamics of entangled melts is clearly impossible—thealgorithms lack stability for the prohibitively large number of integrationtime-steps 6,, and would also require enormous computer time. In thissituation, one must abandon the idea of studying well-equilibrated poly-meric materials of a high degree of polymerization Np in full chemical detail.Several strategies are then conceivable:• Restrict the study to both fairly high temperatures and rather small Np. Although this approach is certainly feasible (see Chapter 8 and Refs 38, 48, 49) and yields interesting information on the behavior on small length scales and small time scales, many problems of interest are excluded. Even on small length scales temperatures close to the glass transition temperature Ts are inaccessible; note, however, that most polymeric sys- tems are studied experimentally at temperatures not far above Ts. Simulations are valuable in particular to complement experiments in a temperature range which would be too high for experiments (e.g., one can study the gas-liquid critical point of alkane chains for Np = 20 to Np = 48, while the chains would chemically decompose at these high temperatures; but nevertheless these critical-point data are a useful input for the equation of state of alkane fluids).• Restrict the study to the small length-scale behavior but abandon the quest for good thermal equilibrium. Of course, in such an approach it is no longer sensible to ask how properties depend on Np, because proper- ties on the length scale of Rg certainly need not be very reliable. This approach is followed in studying the behavior of amorphous polymers in the solid state and their mechanical response (Chapter 5 and Refs 37, 42, 50-58) and certainly is appropriate for studying solid polymers in the crystalline state.5358 The latter problem is not our main concern here, as we concentrate on flexible polymers in the random coil state (solution, melt, amorphous solid). Of course, the "preparation" of the simulation "sample" is then very questionable. Cooling from the melt produces rapidly quenched samples which may differ in many physical properties from their slowly cooled experimental counterparts—at least
23.
COMPUTER S I M U L A T I O N OF P O L Y M E R I C M A T E R I A L S 9one must expect this from experience with coarse-grained models (seeChapter 6 and Refs 59, 60). An elegant alternative is the molecularmechanics technique of generating a dense configuration of amorphouspolymers such that one folds a single (very long) chain back into thesimulation box with the help of periodic boundary condition until thedesired (experimentally given) density is reached, and minimizing thenthe potential energy.50515455 Although the results of this procedure aresometimes extremely encouraging, one must admit that the systematicerrors are uncontrolled: while Monte Carlo (MC) and moleculardynamics methods in principle get better and better the more comput-ing time is invested, e.g., for making cooling slower and slower, it is notclear to what extent this procedure of Theodorou and Suter50 corre-sponds to a physical "sample preparation." This method will not bepursued further in this chapter.Restrict the study to long wavelength properties of the problem byabandoning chemical detail and introduction of a coarse-grainedmodel. It is this approach which will be emphasized in this chapterand many following ones (Chapters 2-4, 6, 7, 9). It is clear that thiscoarse-graining approach makes sense only for "universal" properties,and what universal means depends on the problem under study. Forexample, for dilute polymer solutions one expects that the mean-squaregyration radius of a chain varies with Np as (R^) = CPN^ forNp —*• oo, where the exponent v for good solvents is universal, i.e.,independent of the chemical nature of both polymer and solvent,while the prefactor Cp clearly is not. In a coarse-grained model of apolymer chain we can integrate n chemical monomers into one effectivesubunit (cf. section 1.3) and thus consider an equivalent chain ofN= Np/n "segments." While we still expect (R2g)1/2 = CW, the explicitrelation between C and Cp is lost; while it is known that the exponent vfound from the coarse-grained model coincides with the exponent v ofreal polymers, the prefactor Cp cannot be predicted from the coarse-grained model. Similarly, if we consider unmixing in polymer blends wecan consider the exponent (3 describing the shape of the coexistencecurve (binodal) between the unmixed phases (Chapter 7; see also Refs21, 23, 61-63), the resulting crossover from Ising-like critical behaviorto mean-field-like critical behavior when N increases,23 and consider thequestion how the critical temperature TC(N) scales with TV in a symme-trical polymer mixture ("symmetrical" means N& = Ns = N for bothtypes (A, B) of polymer chains). However, we cannot predict the abso-lute location of Tc (N) nor explain why one pair of polymers (A, B) suchas polystyrene-polymethylvinylether64 has a lower critical point whileanother pair such as polyisoprene-poly(ethylene-propylene) has anupper critical solution temperature (UCST).65
24.
10 INTRODUCTION Thus important goals of molecular simulations, namely predicting physi-cal properties of particular materials quantitatively from a knowledge ofatomistic potentials, to a large extent is lost; however, as emphasizedabove, this consequence is inevitable due to the complexity of polymericsystems. Nevertheless, polymer science is rich with questions which areuniversal, as discussed above, and the large size of polymer coils and thefact that by variation of Np one has a control parameter at hand whichleaves all chemical details invariant (at least to a good approximation) areplausible good reasons that this should be expected. Of course, for problemssuch as the glass transition66 presumably both the behavior on small scales(atoms trapped in "cages" formed by their environment67) and on largescales (relaxation due to cooperatively rearranging regions68) is simulta-neously important—neither the coarse-grained modeling (Chapter 6;References 59, 60, 69) nor the atomic modeling (Chapter 5; Refs 37,39-42) then should be expected to be fully satisfactory! While first attemptsto reintroduce atomistic information from quantum-chemical calculations45into coarse-grained models70"72 look encouraging, more work clearly isnecessary to show that the errors in this approach really are under control.1.2 Survey of simplified modelsThere is no unique way to construct coarse-grained models of polymersystems. In fact, the choice of model very much depends on the physicalproblems that one may wish to address, and also many details are fixedfrom the desire to construct computationally efficient simulation algo-rithms.2773"77 Thus many variants of models for polymer chains exist,and there may still be the need to invent new ones! This section is alsonot intended to be exhaustive, but rather restricts attention only to themost common models which are widely used in various contexts, as willbecome apparent in later chapters of this book.1.2.1 Off-lattice modelsIn section 1.1.2 it was already mentioned that one may wish to simplifymodels for polymers such as polyethylene by replacing CH2 groups by"united atoms." If we simplify the problem further, replacing n successiveCH2 groups by an effective bond between some effective units, we may endup with a model of the type shown78 in Fig. 1.3. In the model of a freely jointed chain (Fig. 1.3[a]) each polymer hence ismodeled by a succession of N rigid bonds of length i jointed together atarbitrary angles. The steps of the Monte Carlo procedure then consist inrotations of beads. For example, bead i is rotated by a randomly selectedangle <p; from its old position to its new position. If the chains are treatedas completely noninteracting, the static and dynamic properties of such a
25.
SURVEY OF SIMPLIFIED MODELS 11Fig. 1.3 Off-lattice models for polymer chains. In the freely jointed chain (a) rigid links oflength (. are jointed at beads by dots and may there have arbitrary angles with each other.The stochastic chain conformational changes are modeled by random rotation of bonds aroundthe axis connecting the nearest-neighbor beads along the chain, as indicated. The new positionof a bead ; may be chosen by assigning an angle (pi chosen randomly from the interval[—A<p, +Ay?] with A<£> < TT. For the simulation of melts, the freely jointed chain is often sup-plemented by a Lennard-Jones type potential (d) between any pairs of beads.80 An alternativemodel is the pearl necklace model (b), where the beads are at the center of hard spheres ofdiameter h, which must not intersect each other. By varying the ratio h/t one can control tosome extent the persistence length of the chain. This model has also proven useful for thesimulation of melts.82 Still another alternative is the bead-spring model (c), which has alsobeen used both for MC simulations as indicated7677 and for MD simulations for solutions8384and melts.8586 (From Binder.78)model are trivial: the configurations of the chains for N large are Gaussiandistributed, and their relaxation is described by the simple Rousemodel.1779 Of course, one can introduce into this model various interac-tions, such as a Lennard-Jones (LJ) interaction between all beads (see eq.[1.3]) and/or a potential controlling the angle between subsequent bonds
26.
12 INTRODUCTIONalong a chain, etc. These potentials then enter the transition probability W((fi) = Mm{exp(-6J^/kB T), 1}, where 6Jf is the energy change producedby the rotation with tf/. According to the standard Metropolis10"1281sampling, the trial move is only carried out if W((pi) exceeds a randomnumber £ distributed uniformly in the interval from zero to one, sincethen one generates an ensemble of configurations (when equilibrium isreached) distributed according to the canonical Boltzmann weights. One can also set the transition probability to zero if the attempted moveleads to some intersection of bonds, in an attempt to simulate entanglementrestrictions as they operate in the dynamics of polymer melts.80 Forbiddingsuch intersections thus takes into account that in the course of their motionschains cannot cross each other. However, the resulting algorithm is ratherslow and has been applied to very short chains only.80 While at high tem-peratures (using an LJ interaction) surprisingly it was found that even in adense melt the chains relax according to Rouse dynamics,17 at low tempera-tures the chains were frozen into a glass-like configuration.80 The pearl necklace model (Fig. 1.3[b]) is a somewhat more useful model,although it is strictly athermal; but, by a proper choice of the ration h/f.between the radius h of the excluded volume sphere around each bead andthe bond length I, one can ensure82 automatically that chains cannot crosseach other if they respect excluded volume restrictions (no spheres areallowed to overlap apart, possibly, from subsequent ones if one choosesl/2<h< I). The most popular and efficient off-lattice models are of bead-spring type(Fig. 1.3[c]) and are not only used for MC but also for MD and Browniandynamics (BD) simulations.7767783"8687"94 It often is advantageous not touse a simple harmonic potential for the bond lengths as in eq. (1.2) butrather allow only a finite extensibility of the chains. In the MD work oneworks with the so-called FENE potential95where one typically chooses the constants k, £max in relation to the para-meters e, a of the LJ potential between the effective beads (eq. [1.3]) as£max = l.Sor, k= 30e/cr2. Note also that one often7683"86 does not workwith the full LJ potential but with an LJ potential that is cut off and shifted,to avoid a ^-function singularity of the force at the cut-off:Choosing7 rc = 21/V the potential is purely repulsive and also the force isnonsingular at r = rc. Note that eq. (1.7) acts between all pairs of beads,including bonded ones.
27.
S U R V E Y OF S I M P L I F I E D M O D E L S 13 With this choice of potentials it is also automatically ensured that anintersection of bonds (in the course of MD or BD simulations) is prevented.For MC simulations, a slightly different choice of potentials was recentlyproposed,76 namelychoosing the same non-bonded potential as in eq. (1.7) and £max = rc,4nin = 0.4 Cax, 4 = 0.7 £max, k/kBT= 10, kBT/€ = 10. With this choice ofparameters, chain intersection also is practically forbidden even if one useslarge attempted displacements of the effective monomers (in each update, amonomer is attempted to be displaced into a randomly chosen direction andthe step width is chosen randomly from a cube with linear dimensions equalto £max, the old position being in the center of the cube). This model can besimulated rather efficiently by applying link-cell methods.87696 Due to thelarge value of the ratio k/ks T one probes in practice only the harmonic partof the potential eq. (1.8), the cut-off at lt = £mjn, ^max has very little effect onthe properties. Choosing a model with purely repulsive interactions one expects neitherthe occurence of a G-temperature in solution, nor a reasonable equation ofstate in the melt (note that in recent MD works8497 solvent molecules areincluded explicitly while in MC simulations one simply reduces the densityof monomers in the box7677 and reinterprets density as the volume fractionof monomers in the solution). Since the LJ potential (eq. [1.3]) for a coarse-grained model lacks any fundamental quantum-chemical foundation, onemay choose any other short-range potential if this is computationally con-venient. With this reasoning, Milchev et al.17 have proposed to use a Morsepotentialwhich has a rather sharp minimum at r = rm;n if one takes a large. Choosinga = 24, rmin = 0.8 (in units of lengths where lmax = 1), one sees that UM (r)/eis essentially zero for r > 1.25 rmn = 1, i.e., the same link-cell techniques canbe applied as in the purely repulsive case. Indeed in this model the 0-pointhas been located and the full regime of concentrations (from dilute solutionto dense melts) has been found accessible, both in the regime of the 0-pointand in the good solvent regime. Finally it should be mentioned that in the MD work it is advantageousnot to choose a strictly microcanonical ensemble (where velocity rescalingsare needed to fix the desired temperatures89) but rather to introduce also acoupling to a heat bath.83 Thus the equations of motions that are integratedare
28.
14 INTRODUCTIONwhere m is the mass of the effective monomer, f/ its position, t the time, #f ,-the total potential energy of monomer i (this may include external poten-tials, of course), F is a bead friction that couples the monomers to the heatbath, and 0(0 describes the random force acting on bead i. This randomforce is related to the friction coefficient via a fluctuation-dissipation rela-tion,assuming Gaussian white noise. More details about the MD approach canbe found in Chapters 3, 4 and 9; here we only mention that this modeldefined by eqs (1.6), (1.7), (1.10) and (1.11) is not restricted to linear poly-mers, but is easily extended to both star polymers9899 and polymer net-works.100"102 Note that the dynamical properties of the model are affectedby the random forces at least at large times; but this problem can be avoidedby using eqs (1.10) and (1.11) only to generate an equilibrated ensemble ofstarting configurations for strictly microcanonical MD runs.84 This is onlyof relevance, if one studies effects of hydrodynamics.84 Finally, one obtainsthe BD approach considering the overdamped limit (strong friction) bysimply omitting the inertial term (wi^?) in eq. (1.10). The advantage ofthe BD approach is that it is most closely related to the theoretical descrip-tions of polymer dynamics, such as Rouse and Zimm models,17 which arecast in a framework of Langevin equations or the (equivalent)Smoluchowski equation for the probability distribution of the configurationof the effective monomers.7.2.2 Lattice modelsThe idea of simplifying the problem even further and representing polymerchains by random walks on a lattice (or, better, by self-avoiding walks[SAW]) is very old and has been used, for instance, for discussing the con-figurational entropy of polymers in solution and of polymer blends.19103104For discussing the configurational statistics of single polymer chains (withexcluded volume interaction) this has been a classic problem for which a richliterature exists that is reviewed in Chapter 2. Here we shall confine our-selves therefore only to a very brief discussion (see also Ref. 2 for moredetails on these models). The simplest model considers a regular lattice where each effective bead ofthe polymer takes a single lattice site, and a bond connecting two beads isjust a nearest-neighbor link on the lattice (Fig. 1.4).105~113 Since each latticesite can at most be occupied by one bead, the walk cannot intersect itself (orother walks, respectively) and thus an excluded volume interaction is auto-
30.
16 INTRODUCTIONmore complicated. It is also clear that the algorithm will have a very smallacceptance rate at high volume fraction (f> of occupied sites, since the vacantsites needed for an acceptable move are then very rare (this holds even moreso if one includes additional moves which need even more vacancies115). Another problem with the algorithm of Fig. 1.4(a) is that it can be provento be nonergodic113116117: one can easily find locally compact configura-tions of a chain that cannot relax by the motions shown. Since the algorithmmust satisfy detailed balance, of course, the chain cannot get into theseconfigurations from other, nonblocked, configurations, and thus there is apart of the configurational space that simply is not included in the samplingat all! Although this does not seem to be a problem in practice (comparingdata from different types of algorithms yields equivalent results within thestatistical errors62), one must be aware of this drawback if one either tries tostudy much longer chains or tries to improve significantly the accuracy. Due to the need for sufficient vacancies this algorithm has only beenused6162114 for volume fractions </> < 0.8. The "slithering snake algorithm(Fig. 1.4[b]), on the other hand, needs only one vacant site near a chain endfor a successful move and thus can be used for significantly denser systems(<t> = 0.976 was successfully used118119). It also suffers from the problem thatit is not strictly ergodic,117 although again these "blocked configurations"do not seem to affect the accuracy to a practically relevant extent.2 If one isinterested in static chain properties, an advantage of the slithering snakealgorithm is that it relaxes distinctly faster2120 than the generalized Verdieralgorithms. The latter (for single chains) produce a Rouse-type1779 relaxa-tion and must be used if one is interested in dynamical chain properties,whereas the slithering snake move (in which one tries to remove a randomlychosen end-link of a chain and add it in a randomly chosen direction on theother chain-end) obviously has no counterpart in the dynamics of realchains. For most static properties of single chains, the algorithm of choice isclearly the pivot algorithm110"113 (Fig. 1.4[c]), where one randomly choosesa link in the chain and then rotates this link together with the rest of thechain to a randomly chosen new orientation on the lattice. Of course, thenew configuration is accepted only if it does not violate the excluded volumeconstraint. The advantage of such moves is that one rapidly generates newchain configurations, which are not "dynamically correlated" with theirpredecessors.21178113 Of course, this algorithm cannot then be used for astudy of dynamical properties of chains, and it is also not useful for densepolymer systems. An algorithm that incorporates large nonlocal moves of bonds and worksfor dense polymer systems (even without any vacancies, < / > = ! ) is the"collective motion" algorithm121"123 where one transports beads fromkinks or chain ends along the chain contour to another position along thechain, for several chains simultaneously, so that in this way this rearrange-
31.
S U R V E Y OF S I M P L I F I E D M O D E L S 17ment exchanges some of the sites taken by their beads. Due to the nonlocalcollective rearrangements of several chains, the algorithm is rather compli-cated and is not straightforwardly suited to vectorization or parallelization.Thus only if the vacancy concentration (f>v = 1 — 0 is very small, does thisalgorithm have an advantage (in comparison with the algorithms of Figs1.4[a,b]) since these other algorithms then have a very small acceptance rate.Also one clearly cannot associate a physical meaning to the time variable inthis algorithm, although this sometimes was attempted.121 Since real poly-mer melts do have a nonzero compressibility, which in the framework ofsimple lattice models (SAWs on the sc lattice) is roughly reproduced with avacancy content124 of about (j>v = 0.1, one also should not claim that amodel with strictly 0V = 0 is more realistic than the models that containvacancies. If one defines a van der Waals density in terms of the repulsivepart of the interatomic potential in real polymers, one obtains a van derWaals density of only about 50%. Thus, in our view, the collective motionalgorithm poses more disadvantages than advantages. The lattice algorithm that is now most widely used for the simulation ofmany-chain systems is the bond fluctuation model (Fig. 1.5).73>125~128 It hasbeen used to model the dynamics of both two-dimensional125 and three-dimensional polymer melts,127128 the glass transition 129 also Chapter 23 63 (see6))59,6o,69-72 polymer blends (see also chapter 7), polymer net-works,130 gel electrophoresis,131 polymer brushes (see Chapter 9) and soon, and it was attempted to map it on to real materials,70"72 This model isin a sense intermediate between the simple SAW model of Fig. 1.4 and theoff-lattice models (Fig. 1.3), because the vector that connects two monomerscan take 36 values (in d = 2 dimensions) or 108 values (in d = 3 dimensions),rather than four or six (square or simple cubic lattice, respectively). Whilethus the continuum behavior is almost approximated, one still enjoys theadvantages of lattice algorithms (integer arithmetics, excluded volume ischecked via the occupancy of lattice sites, etc.) The restriction in the allowedbond lengths assures that the excluded volume interactions simultaneouslymaintain the constraint that bonds cannot cross each other in the course ofrandom motion of the monomers. The fact that there is a single type ofmotion that is attempted (random displacement of an effective monomer,i.e., an elementary plaquette of the square lattice d— 2] or an elementarycube of the simple cubic lattice [d = 3] in a randomly chosen lattice direction)allows very efficient implementations of this algorithm, including vectoriza-tion.126 This algorithm also suffers less from ergodicity problems than thealgorithms of Figs 1.4(a) and (b), although it is not strictly ergodic either. Forsingle chains, from this algorithm a Rouse-model type dynamicsresults,177379127 as desired, while in dense melts (i.e., systems wherecj) > 0.5127) a crossover occurs127128 from Rouse-like behavior (for N < 50)to reptation-like behavior1617132 for long enough chains that then aremutually entangled.
32.
18 INTRODUCTIONFig. 1.5 Schematic illustration of the bond fluctuation model in three dimensions. An effectivemonomer blocks a cube containing eight lattice sites for occupation by other monomers. Thelength t of the bonds connecting two neighboring cubes along the chain must be taken from theset 1 = 2, /5, /6,3, vTO. Chain configurations relax by random diffusive hops of the effectivemonomers by one lattice spacing in a randomly chosen lattice direction. (From Deutsch andBinder.129) While at first sight it may seem pathological that the length of an effectivebond may vary over a wide range (2 < t < vT3 in d = 2, 2 < I < VlO ind = 3), this is natural when one recalls that each effective bonds represents agroup of n C-C bonds along the backbone of the chemically realistic chain(Fig. 1.1), and, depending on the conformation of this group its end-to-enddistance may vary significantly. This idea will be explored in more detail inSection 1.3 by attempting to develop effective potentials for the length £ ofeffective bonds and the angle 6 between two consecutive such bonds fromthe underlying microscopic (i.e., chemically realistic) model of the polymerchain. The fact that one can have such potentials for the length of the bondvector easily allows the modeling of the glass transition of polymer melts(see Chapter 6) which is less straightforward on the basis of the model ofFig. 1.4. Finally we end this survey by emphasizing that there is no unique answerto the question "which is the best model of a polymer chain"; depending onthe types of application and the questions that are asked different modelsand different algorithms may be useful, and there is still room for inventingnew algorithms. For example, for a study of ionomers, where chains sticktogether at certain sites due to electrostatic forces, it was advantageous touse an algorithm which allowed the "stickers" to exchange partners and to
33.
T A K I N G THE IDEA OF C O A R S E - G R A I N I N G L I T E R A L L Y 19translate parts of the chain rigidly.133 Polymer chains in d= 2 dimensionscan be simulated by a particularly fast but locally very unrealistic algo-rithm.7475 We also emphasize that we have discussed dynamic algorithmsonly—there also exist useful algorithms to construct SAW configurations bygrowing them in a stepwise manner by various techniques. For a review ofsuch "static" methods, see Ref. 2 and Chapter 2. These static methods areparticularly useful if one wishes to estimate the number of configurations ofthe polymers and the associated exponents. Note that such techniques arenot only applicable to linear polymers but can be extended to differentpolymer architectures, such as many-arm star polymers.1341351.3 Taking the idea of coarse-graining literallyIn the previous section, we have seen that a variety of crudely simplifiedmodels of polymer chains is available. In this section we discuss the extent towhich such models can be connected with more microscopic, chemicallyrealistic descriptions, and how one should proceed when comparing resultsfrom different model calculations with each other.1.3.1 Effective potentials for the bond fluctuation modelThe coarse-grained model can be obtained by combining n successive cova-lent bonds along the backbone of a polymer chain into one effective segment(see Fig. 1.6 where n = 3 is chosen). In principle, such a procedure can becarried out for any polymer (e.g., in Refs 45, 70-72 an application to bis-phenole-A-polycarbonate (BPA-PC) is discussed). In order to make closecontact with reality, one may wish to carry out this mapping such that thelarge-scale geometrical structure of the polymer coil is left invariant, i.e.,properties such as the gyration radius of the coil and the probability dis-tribution of its end-to-end distance should be the same for the coarse-grained model in Fig. 1.6 as for the chemically detailed model. The idea of Refs 70-72 is that this invariance of long wavelength proper-ties is indeed realized if we introduce suitable potentials in the coarse-grained model which control bond lengths of the effective bonds, anglesbetween effective bonds along the sequence of the coarse-grained chain,etc. In practice, it was proposed70"72 to use harmonic potentials both forthe length i of an effective bond and for the cosine of this effective bondangle, i.e.,where UQ, IQ, V0, cose0 are four adjustable parameters (which may dependon the thermodynamic state of the considered polymer melt, of course, i.e.,temperature and pressure). It is thought that these potentials "mimick" the
34.
20 INTRODUCTIONFig. 1.6 Use of the bond fluctuation model on the lattice as a coarse-grained model of achemically realistic polymer chain (symbolized again by polyethylene). In the example shownn = 3 covalent bonds form one "effective bond" between "effective" monomers: chemicalbonds 1,2,3 correspond to the effective bond I, chemical bonds 4,5,6 to the effective bond II,etc. (From Baschnagel et a/.,45)effect of the potentials.of the microscopic model, such as eqs (1.!)-(!.3)describing potentials for the lengths of chemical bonds and their bondangles and torsional angles. So the information on these potentials andhence the chemical structure is not completely lost in the coarse-graining,but at least some caricature of it is still found in the simplified model (Figs1.5, 1.6) via the potentials in eq. (1.12). We do not only wish to map the behavior on large length scales but alsoon large time scales. Since a move of an effective monomer as shown in Fig.1.5 requires transitions from one minimum of the torsional potential toanother, on the scale of the chemically realistic model (Fig. 1.2), informationon the barrier heights of this torsional potential must also be incorporatedinto USK((-), J/eff(0), since these potentials govern the transition probabilityof the Monte Carlo sampling process.136 The corresponding explicit con-struction of the parameters in eq. (1.12) from the available quantum-chemical information on potentials such as written in eqs (1.1)™(1.3) israther tedious and difficult136 and will not be discussed further here. If the potentials Uef{(£), F e ff(e) are known, their basic effect will be togenerate distributions according to the Bolt/mann weightand similarly for Pn(Q). These distributions can also be obtained directlyfrom the chemically realistic model of an isolated chain (Fig. 1.7)4345 andchecking that the model distribution (eq. [1.13]) represents the actual dis-tribution faithfully enough hence is an important consistency check of thedescription. One can infer that for n = 5 (which is a reasonable choice, since
35.
T A K I N G THE IDEA OF C O A R S E - G R A I N I N G L I T E R A L L Y 21Fig. 1.7 (a) Distribution function P5(t) vs. t (measured in units of to = 1.52A) for n = 5 sub-sequent CH2 units integrated into one effective bond. Three temperatures are shown as indi-cated. The nonbonded LJ interaction was only included up to the seventh neighbor along thechain, to ensure Gaussian chain statistics at large distances, as it occurs in dense melts where theLJ interactions are screened out. (b) same as (a) but PS (9) plotted vs. angle 6 between subse-quent effective bonds. (From Baschnagel et al. )7 must be large enough to include several torsional degrees of freedom, butsmall enough to still contain information on the scale of the persistencelength) the distributions for Pn(l), Pn(cosQ) are indeed reasonably wellipproximated as Gaussian: this finding, in fact, was the motivation for
36.
22 INTRODUCTIONthe choice of the simple quadratic potentials, eq. (1.12). The weak tempera-ture dependence that one can see in Fig 1.7 simply reflects the gradualtendency of the PE chain to stretch (increase of the persistence length andthe characteristic ratio C^ = lim (R2)/Np(fi)) as the temperature is low- fered., Na—>00 A consequence of the mapping in Fig. 1.6 being taken literally is that the(otherwise not explicitly defined) length and time scales of the coarse-grained model get a physical meaning. For example, for BPA-PC oneobtains (when one monomer with 12 chemical bonds along the backboneis mapped onto three effective bonds) that a lattice spacing at T = 570 Kcorresponds to 2.3 A, and one Monte Carlo step per monomer (attemptedmonomer hop, which has an acceptance rate of about 1 % only due to therestrictive potentials) corresponds to 10~13 s, a successful hop occurs atabout a time of 10~" s. Obviously, this is physically reasonable, and rele-vant information has been lost on a very small length scale (< 3 A) only.Choosing70"72 lattices of a typical linear dimension of L = 40 latticespacings then means that systems of a linear dimension of about 102Aare simulated, which clearly is somewhat larger than the sizes accessible inthe study of microscopically realistic models.36"42 50"55 Note that the largestlattice used so far23 (for the study of the critical behavior of polymer blends,see also Chapter 7) used L = 160 and did contain 256000 effective mono-mers, which with n = 5 (Fig. 1.7) would correspond to 1 280000 CH2 units(and N = 512 would translate into Np = 2560, a reasonably large degree ofpolymerization23).1.3.2 How different coarse-grained models can be comparedFrom the previous discussions it should be clear that there is no uniquemodel description of a polymer chain system; in fact, for different physicalquestions somewhat different coarse-grained models are optimal. For exam-ple, while the bond fluctuation model73126"129 is very well suited to the studyof polymer melt dynamics,125"128 polymer blends,2363 the glass transi-tion,596069 polymer brushes in good solvents137 and so on, for otherproblems it is less well suited: lattice structure artefacts appear in thestudy of collapsed polymer brushes in bad solvents138 and in models fordense lipid monolayers at the air-water interface139; in the presence offrozen-in obstacles, locked-in chain configurations must be expected.76For such problems, off-lattice models clearly are better suited. How thencan results from different models be combined and compared quantita-tively? This question is similar to the question of how to compare simulationsand experiment85 or to compare Monte Carlo work with MD work,127 ofcourse. But a need for such a conversion arises even when somewhat differ-ent Monte Carlo models need to be compared. This question was addressed
37.
T A K I N G THE IDEA OF C O A R S E - G R A I N I N G L I T E R A L L Y 23by Milchev et a/.76 who compared data for their off-lattice bead springmodel, where results for various chain lengths N and volume fractions <j>were obtained, to results for the bond fluctuation model127 where data for avariety of values for chain lengths N and volume fractions <j> are available.While on the lattice the term "volume fraction" is not ambiguous, it issimply the percentage of lattice sites blocked by the effective monomers;there clearly is some arbitrariness for the off-lattice case. Gerroff et a/.7677define it as the number of effective monomers per cell of size £^ax: thus <j>(unlike </>) can even be larger than unity, and the question of translating thevariable </> to the variable (j> arises. Similarly, the models may exhibit differ-ent degrees of local chain stiffness, and hence there also is no one-to-onecorrespondence between N and N. This point is sometimes overlooked in thecomparison of different models.140 Gerroff et al.76 argue that it is the universal scaling limit that can beextracted from different models and which must be identical; so, whenone considers the scaling limit N —> oo, <f> —> 0 (or N —> oo, <j> —> 0), onemust obtain the same scaling function for (R*(<t>)} / (&((j> = 0)} versusN/Nb0b(<t>) oc jV^1^3""1), which describes the crossover from the dilute tothe semidilute limit (Fig. 1.8). This scaling function is universal (for goodsolvents), because on large length scales compared to microscopic lengthscales (such as bond lengths) the chains are self-similar. The only relevantlength scale for the distribution of intramolecular distances can be taken tobe the radius of gyration measured in units of the microscopic length scale. Differences in the nonuniversal prefactors like the persistence length leadto the necessity of mapping different chain lengths onto one another. In thedilute limit, we write for the mean square gyration radius (J?2,)where C is a dimensionless (nonuniversal) constant and24 v = 0.59.Similarly, for the bond fluctuation model an analogous relation holds:Now the two models are mapped onto each other defining N = aN andfixing the conversion factor a such that the amplitude factors in eqs(1.14a) and (1.14b) then are equal, Ca2v = CBF- From the numerical resultsC= 0.24, CBF = 0.164 it was found that a & 0.274, i.e., the range fromN = 8 to N = 64 was mapped to a range from N K 11 to N « 88 in thebond fluctuation model. The conversion from <f> to (j> is achieved similarly, noting that for (f> 3> <p* ((/)*is the overlap concentration in the solution, defined by NE(<J>*) = N whereNB(4>) is the number of segments per blob, i.e., N/(R2S)3/2 = 4>* oc AH3"-1))the behavior of Rs is classical:
38.
Fig. 1.8 (a) Log-log plot of the reduced mean square gyration radius, (/?g(^)}/{/{|(0)), vs.rescaled chain length (N - l)^3)1^3""1, where ^ is the root mean-square bond length, and thetheoretical value >24 for the exponent v(y = 0.59) is used. All data refer to a bead-spring modelwith stiff repulsive Lennard-Jones interaction, as described in Section 1.2.1 (Eq. [1.7]). (b) Sameas (a) but for the bond fluctuation model. In both (a) and (b) the straight line indicates theasymptotic slope of the crossover scaling function, resulting from eq. (1.15). (From Gerroffet al.)24
39.
T A K I N G THE IDEA OF C O A R S E - G R A I N I N G L I T E R A L L Y 25or alternatively in the bond fluctuation model Using then N = aN and <p = /3<j> and requiring that {jR2}/{,£2} is the samein both models yields C^F = Ca/H2""1^3""1) as a condition that bothscaling functions in Figs 1.8(a) and (b) superimpose. One finds for themodel of Gerroff et al.16 that /3 = 0.3, i.e., $ = 1.5 in the off-lattice modelcorresponds to <j> =• 0.5 in the bond fluctuation model. It is possible to carry over such considerations to dynamic quantities aswell (see also Chapter 4). This is of interest, of course, for comparing theefficiency of different algorithms. It then does not make sense to comparethe time it takes to carry out one Monte Carlo step (MCS), since step widthand acceptance rate of the moves also matter: what must be compared arephysical relaxation times. One such relaxation time for a polymer chain canbe defined128 as the time r needed for an inner monomer of a chain to travela distance equal to the gyration radius. Defining mean square dynamicdisplacements of inner monomers as follows,it also is of interest to consider an analogous quantity in the center ofmass system of the chain (fcu(t) being the position of its center of massat time ()127>128and the mean-square displacement of the center of mass itself,Finally, mean-square displacements of monomers at the free ends of thechains are defined asNow relaxation times T, TI, T3, r$ can be defined from requiring thatFigure 1.9 illustrates the variation of these mean-square displacements withtime and the estimation of the resulting relaxation times T, TI, T$, T$ forthree different models: the bond fluctuation model,127128 the off-latticebead-spring model of Gerroff et al.,76 and the molecular dynamics simula-tion of a realistic model for short polyethylene chains (Np = 50) in the melt
41.
T A K I N G THE IDEA OF C O A R S E - G R A I N I N G L I T E R A L L Y 27Fig. 1.9 (a) Log-log plot of mean-square displacements versus time (measured in attemptedMonte Carlo steps per monomer) for the bond fluctuation model at parameters correspondingto a dilute solution (N =20,<f> = 0.075). (b) Log-log plot of mean-square displacement versustime (measured in attempted Monte Carlo steps per monomer) for the bead-spring model ofGerroff et al.76 at parameters corresponding to a dilute solution (<j> = 0.5, N = 16). Broken andstraight lines shows the measurement of (R^) and the mean-square end-to-end distance (J?|),respectively, and the gt(t) are defined in eq. (1.16). (From Gerroff et al..16) (c) Log-log plot ofmean-square displacements versus time (measured in picoseconds) from the MD simulation of64 systems run in parallel containing 20 PE chains with degree of polymerization 7VP = 50 andmelt densities. The mean-square gyration radius is denoted as (S2) in this figure. (From Brownet a/.38)(at temperature T = 500K).38 It is seen that the general behavior is rathersimilar in all three models. Of course, only the chemically realistic model ofBrown et a/.38 has physical scales (picoseconds for time and A for lengths,respectively); the Monte Carlo work of the coarse-grained model measurestime in attempted moves per monomer and length in lattice spacings.Remembering that one MCS may correspond to about 10~13 s in thebond fluctuation model, a time-scale of 103 in Fig. 1.9(a) corresponds toabout lOOps, indeed a comparable time to Fig. 1.9(c). Note that Np = 50(shown in Fig. 1.9[c]) would correspond to about N = 16 in Figs 1.9[a],[b])with a mapping (Fig. 1.6) Np = Nn with « = 3. Remembering that a latticespacing corresponds to about 2.3 A (Fig. 1.9[a]) would imply (7?g) w 200 A,again comparable to the realistic model (Fig. 1.9[c]). Of course, strictly speaking the different models need be equivalent onlyin the scaling limit N —>• oo, 0 -* 0 (for the realistic model of a polymer insolution a different dynamics would then result, described by the Zimmmodel,141 due to hydrodynamic forces mediated by the solvent molecules
42.
28 INTRODUCTION(see also Chapter 3).71784 Only in the absence of solvent molecules may theRouse model result also from an MD simulation83). Another universalregime results for dense melts: then it is the entanglement molecular weightNe of the different models that needs to be mapped for a quantitativecomparison (see also Chapter 4).7>85127 Since Figs 1.9(a), (b) refer to solu-tion while Fig. 1.9(c) refers to a melt, one should not expect more than asimilarity of qualitative character here. Since chains renew their configura-tion only on time scales larger than these characteristic times T, TI, TI, r$,Fig. 1.9(c) provides practical evidence for our estimates of section 1.1.2, thattimes exceeding a nanosecond are needed to equilibrate melts of non-entangled short chains at high temperatures. Only for the coarse-grained models can one so far estimate the variationof the relaxation times over a significantly wide range of N, N (Fig. 1.10).One finds the expected power-law behavior for both models. A particularlyinteresting feature is found when one compares the absolute value of therelaxation times for the same chain length: e.g., for N = 3Q we haver K> 1200 in the off-lattice model but r ~ 3600 in the bond fluctuationmodel. Thus the off-lattice model needs a factor of three less MCS toreach the same physical relaxation time. This fact partially offsets the dis-advantage that the off-lattice algorithm performs distinctly slower. Thus the general conclusion of this section is that one must think carefullyabout the conversion of scales (for length, time, molecular weight) when onecompares physical results from different models, or the efficiency of variousalgorithms. It is hoped that the above examples serve as a useful guideline ofhow to proceed in practice.1.4 Selected issues on computational techniquesIn this section are briefly reviewed some technical problems of the simula-tion of dense many-chain systems, such as the sampling of intensive vari-ables such as chemical potential, pressure etc., but also entropy, which arenot straightforward to obtain as averages of "simple" quantities. Some ofthe standard recipes developed for computer simulation of condensedphases in general8"13 have difficulties here, due to the fact that the primaryunit, the polymer chain, is already a large object and not a point particle.But knowledge of quantities such as the chemical potentials are necessary,e.g., for a study of phase equilibria in polymer solutions.421.4.1 Sampling the chemical potential in NVT simulationsThis problem has been brilliantly reviewed by Kumar in a recent book142and hence we summarize only the most salient features here. For smallmolecule systems, sampling of the chemical potential rests on the Widomtest particle insertion method143
43.
S E L E C T E D ISSUES ON C O M P U T A T I O N A L T E C H N I Q U E S 29Fig. 1.10 Log-log plot of relaxation time T vs. chain length N, for the bead-spring model withsoft Lennard-Jones repulsion76 and the bond fluctuation model.128 Open circles (and left ordi-nate scale) refer to off-lattice model at <j> = 0.0625, full dots (and right scale) to the bondfluctuation model at </> = 0.05 (data taken from Ref. 128). Straight lines indicated the powerlaws r oc N2, where the exponent z = 2.3 or 2.24, respectively, is reasonably compatible withthe theoretical prediction16- z = 2 ^ + 1 KI 2.18. Insert shows the ratio T$/T. It is seen that bothmodels give mutually compatible results for the JV-dependence of this dimensionless ratio(which should settle down at some universal constant for N —> oo). In this figure the distinctionbetween N and N (which is only a rather small shift on the logarithmic scale) is disregarded.(From Gerroff et a/..76)where A/x is the chemical potential difference relative to the chemical poten-tial of an ideal gas at a same temperature and density, F^- is the Helmholtzfree energy of a system containing Jf particles, and { ... )^ represents acanonical ensemble average. This test particle insertion method involves theinsertion of a ghost particle into a frozen equilibrium snapshot of a systemcontaining Jf particles, and U denotes the total potential energy experi-enced by this test particle. Averaging the appropriate Boltzmann factorover many different configurations (frozen snapshots) of the system, thechemical potential is obtained from eq. (1.18), and this method works
44.
30 INTRODUCTIONwell in practice for small molecule fluids (for examples see Refs 144, 145).Now, for polymers the insertion of a polymer in a frozen equilibrium snap-shot has a very low acceptance probability, and this probability decreasesexponentially with increasing chain length. Hence this method has beenrestricted to N < 20 for lattice models146147 and to N < 15 for pearl neck-lace off-lattice chains.148"151 Several schemes have been devised by various authors, some of them rely-ing in one form or another on the biased sampling scheme of Rosenbluth andRosenbluth152 and others on thermodynamic integration methods.8"13 TheRosenbluth-Rosenbluth method was devised originally as a sampling schemefor generating configurations of SAWs on a lattice (see Chapter 2) that avoidsthe "attrition problem" (i.e., the loss of chain configurations that have to beabandoned because they are overlapping). In this scheme one grows the SAWstep by step and checks at each step which sites are available for the next stepwithout violating the SAW constraint. One of these steps is then selected atrandom. Since relative to the simple sampling of SAWs this method creates abias,2153 one has to keep track of the probability of each configuration rela-tive to the unbiased simple sampling, and weigh the generated chain config-urations with this probability accordingly. An approximate generalization of this method to multichain systems dueto Meirovitch is called "scanning future steps".154155 Suppose we wish toput Jf chains of N monomers each on a simple cubic lattice of L3 sites. Astarting point for the first polymer is selected out of the L3 lattice sites withprobability L~3 and occupied by a monomer. The first chain is then grownby a method where one scans b future steps: once the first k monomers havebeen placed, one counts for each of the six neighbors of the last site theallowed continuations consisting of b further steps (for the monomers k + 1to k + b) which start at this last site. The probability for selecting one of thesix neighbors is chosen proportional to the number of allowed continuationsstarting at this site. Then the (k+ l) th monomer is placed on the selectedsite, and so on. In this way one has to place N monomers for the firstpolymer. If at any step no continuation is possible, the construction isabandoned and one starts a new polymer from a new starting point. Once the first polymer is generated on the lattice, a starting point for thesecond polymer is selected out of the remaining L3 — N sites with equal prob-ability, and the further N - 1 monomers of the second polymer are placed onthe lattice according to the same method as described above. The excludedvolume interaction is taken into account with respect to the first chain and thealready grown parts of the second chain. This procedure is continued until thedesired number of chains on the lattice has been reached. The fraction of successful construction attempts is not an exponentiallydecreasing function of the number of chains Jf, but stays approximatelyconstant at unity until a critical value that depends on N and Z>.154~156 Thelarger N and/or jV is, the larger one should use b; however, since the
45.
S E L E C T E D ISSUES ON C O M P U T A T I O N A L T E C H N I Q U E S 31number of future steps that need to be scanned increases with b, in practiceone is again limited to rather small N. Since one knows at each step of the construction of a configuration theprobability for selecting a lattice site for the next monomer, one can multi-ply all these single step probabilities in order to obtain the probability Pv ofconstructing the multiple chain configuration v. Then the partition functionZ is estimated from a sampling of the inverse of PvFrom the partition function the free energy Fjf follows and hence all ther-modynamic quantities of interest can be estimated (entropy, chemical poten-tial, osmotic pressure...). Ottinger156 applied this technique to test theosmotic equation of state for dilute and semidilute polymer solutions forN < 60. Extension of this technique to off-lattice systems has also beenmade.157158 A variant of the Rosenbluth-Rosenbluth method tailored to overcomethe test chain insertion problem in the Widom method143 (Eq. [1.8]) has beendeveloped by Frenkel et a/.159"163 and is known as configurational biasMonte Carlo (CBMC). They rewrite eq. (1.18), using the fact thatU = ^2jLi Uj,jf+i> the energy of a test chain of length N inserted into asystem of Jf other chains, can be written as a sum of energies Uj^+ ofthe individual beads,Equation (1.20) suggests inserting the test chain bead by bead, and to over-come the sampling problems created by the relatively small probability ofrandomly inserting a test chain, without overlap, in a frozen snapshot of thesystem at liquid-like densities. Frenkel et a/.159"163 use a biased insertionprocedure which favors low energy conformations of the inserted chain.The first bead is inserted at random and the interaction energy of thisbead with the rest of the system (Utjy+) tabulated. Then k( < k < oc)trial positions are generated for the next bead, obeying any geometric con-straints imposed by chain architecture. The energy of each of these trialpositions (t4,/r+i) K calculated, and one position (I) is randomly chosenaccording to a weight Wf,Subsequent beads of the test chain are grown similarly until one arrives atthe desired chain length.
46.
32 INTRODUCTION One now has to correctly weigh the states generated by this biased inser-tion procedure when one calculates the chemical potential from eq. (1.20):since we generated states of the canonic ensemble modified with a weightingfunction, w, we have to correct for this weighting function as follows142163where (/~o) represents the desired average of an observable/in the canonicensemble, and { . . . ) in the weighted ensemble. Applying this to eq. (1.20)yieldsnoting that no bias needs to be corrected for the first segment. Substitutingeq. (1.21) in eq. (1.23) finally yieldsIt is important to emphasize the distinction between the CBMC method159-163 ancj jj^ originai Rosenbluth scheme.152 As is well known,153 the lattergenerates an unrepresentative sample of all polymer conformations, i.e., theprobability that a particular conformation is generated is not proportionalto the Boltzmann weight of that conformation, and thus one has to correctfor the difference in weights and thus arrives at a biased sampling schemewhich has problems for large N.153 In the CBMC scheme, on the otherhand, the Rosenbluth weight is used to bias the acceptance of trial confor-mations that are generated with the Rosenbluth scheme. Therefore all con-formations occur with their correct Boltzmann weight. This is achieved bycomputing the Rosenbluth weights wiriai and woki of the trial conformationand of the old conformation (in the trial conformation one may regrow anentire polymer molecule or only a part thereof). Finally the trial move isaccepted only with a probability min{wtriai/w0id, !}• As explained byFrenkel,163 this method is also readily applied to off-lattice chains.
47.
S E L E C T E D ISSUES ON C O M P U T A T I O N A L T E C H N I Q U E S 33 At this point, we note that the chemical potential defined from a stepwiseinsertion procedure as described above can also be written asHr(j) being the incremental chemical potential to add a bead to a chain oflengthy— 1. Equation (1.25) is the basis of the chain increment method ofKumar et a/.142164"167 One now can prove166 an analog of the Widom for-mula, eq. (1.18), for /ir(/),where the ensemble that is considered comprises Jf — 1 chains of length Nand one chain of length j— 1, with 1 <j<N. One considers a frozensnapshot of this system, inserts a bead onto one of the ends of thechain of lengthy— 1 and evaluates £/(r/)> the test bead energy. The incre-mental chemical potential fir(j) is then computed by averaging the appro-priate Boltzmann factor over many different realizations of the simulatedsystem. In the end one is interested in p,r(N), of course, so this procedurehas to be carried out for a whole sequence of simulations, where j runsfrom 1 to N. This restricts the technique in practice to relatively shortchain lengths, but the advantage of this scheme in comparison to theCBMC method is that one avoids the sampling problems that biasedsampling methods often inevitably have.153 An alternative method has recently been proposed by Muller and Paul168using the concept of thermodynamic integration. The idea is to circumventthe problem of the vanishingly small acceptance probability for inserting achain respecting excluded volume constraints in a dense system by allowingoverlap of the inserted "ghost chain" with the other chains which are strictlymutually- and self-avoiding. If the ghost chain overlaps with TVo monomers,the statistical weight of the configuration is A^0. One has to carry out thisinsertion many times in statistically independent configurations of themany-chain systems and carry out a sampling of (No(X,4>)} to find theexcess chemical potential of the polymers (relative to an ideal noninteractingpolymer gas): It was found useful to carry out the integration in eq. (1.27) by performingsimulations at about nine distinct values of A, which are used as input into amultihistogram analysis which yields a very good estimate of (A/o(A,(/>))
Be the first to comment